 Nano Express
 Open Access
 Published:
Theory and simulation of photogeneration and transport in SiSiO_{ x } superlattice absorbers
Nanoscale Research Letters volume 6, Article number: 242 (2011)
Abstract
SiSiO_{ x } superlattices are among the candidates that have been proposed as high band gap absorber material in allSi tandem solar cell devices. Owing to the large potential barriers for photoexited charge carriers, transport in these devices is restricted to quantumconfined superlattice states. As a consequence of the finite number of wells and large builtin fields, the electronic spectrum can deviate considerably from the minibands of a regular superlattice. In this article, a quantumkinetic theory based on the nonequilibrium Green's function formalism for an effective mass Hamiltonian is used for investigating photogeneration and transport in such devices for arbitrary geometry and operating conditions. By including the coupling of electrons to both photons and phonons, the theory is able to provide a microscopic picture of indirect generation, carrier relaxation, and interwell transport mechanisms beyond the ballistic regime.
Introduction
SiSiO_{ x } superlattices have been proposed as candidates for the high band gap absorber component in allSi tandem solar cells [1, 2]. In these devices, photocurrent flow is enabled via the overlap of states in neighboring Si quantum wells separated by ultrathin oxide layers, i.e., unlike in the case of an intermediate band solar cell, the superlattice states contribute to the optical transitions and, at the same time provide transport of photocarriers, which makes it necessary to control both the optical and the transport properties of the multilayer structure. To this end, a suitable theoretical picture of the optoelectronic processes in such type of structures is highly desirable.
There are several peculiar aspects of the device which require special consideration in the choice of an appropriate model. First of all, a microscopic model for the electronic structure is indispensable, since the relevant states are those of an array of strongly coupled quantum wells. In a standard approach, these states are described with simple KronigPenney models for a regular, infinitely extended superlattice [3]. The superlattice dispersion obtained in this way can then be used for determining an effective density of states as well as the absorption coefficient to be used in macroscopic 1 D solar cell device simulators. However, depending on the internal field and the structural disorder, the heterostructure states may deviate considerably from regular minibands or can even form WannierStark ladders. Furthermore, the charge carrier mobility, which has a crucial impact on the chargecollection efficiency in solar cells, depends on the dominant transport regime at given operating conditions, which may be described by miniband transport, sequential tunneling, or WannierStark hopping [4], relying on processes that are not accessible to standard macroscopic transport models.
In this paper, the photovoltaic properties of quantum well superlattice absorbers are investigated numerically on the example of a SiSiO_{ x } multilayer structure embedded in the intrinsic region of a pin diode, using a multiband effective mass approximation for the electronic structure and the nonequilibrium Green's function (NEGF) formalism for inelastic quantum transport, which permits to treat on equal footing both coherent and incoherent transport as well as phononassisted optical transitions at arbitrary internal fields and heterostructure potentials.
Theoretical model
In order to enable a sound theoretical description of the pivotal photovoltaic processes in semiconductor nanostructures, i.e., charge carrier generation, recombination and collection, both optical transitions and inelastic quantum transport are to be treated on equal footing within a consistent microscopic model. To this end, a theoretical framework based on the NEGF formalism was developed [5, 6] and applied to quantum well solar cell devices. In this article, we reformulate the theory for a multiband effective mass Hamiltonian, similar to [7, 8], and extend it to cover the phononassisted indirect transitions that dominate the photovoltaic processes in Sibased devices. Furthermore, in contrast to the former case, both photogeneration and transport processes take place within superlattice states, since escape of carriers to continuum states is not possible due to the large band offsets.
Hamiltonian and basis
The full quantum photovoltaic device is described in terms of the model Hamiltonian
consisting of the coupled systems of electrons (Ĥ _{e}), photons (Ĥ _{γ}), and phonons (Ĥ _{p}). Since the focus is on the electronic device characteristics, only Ĥ _{e} is considered here, however including all of the terms corresponding to coupling to the bosonic systems.
The electronic system without coupling to the bosonic degrees of freedom is described by
with
where V _{0} is the heterostructure potential, and U is the Hartree term of the Coulomb interaction corresponding to the solution of Poisson's equation that considers carriercarrier interactions (Ĥ _{ee}) on a mean field level.
The Hamiltonian representations for the interaction terms are obtained starting from the singleparticle interaction potentials. For the electronphoton interaction, the latter is given via the linear coupling to the vector potential operator of the electromagnetic field Â:
with the momentum operator and
where ε_{λq }is the polarization of the photon with wave vector q and energy ħω _{λq }added to or removed from photon mode (λ, q) by the bosonic creation and annihilation operators:
and V is the absorbing volume.
The vibrational degrees of freedom of the system are described in terms of the coupling of the force field of the electronion potential V _{ei} to the quantized field of the ionic displacement [9]:
with the displacement field given by the Fourier expansion:
where the ion equilibrium position is L + κ, with L being the lattice position, and κ being the relative position of a specific basis atom at this lattice site, and are the bosonic creation and annihilation operators for a (bulk) phonon mode with polarization Λ and wave vector Q in the first Brillouin zone. The potential felt by electrons in heterostructure states due to coupling to bulk phonons can thus be written as
where r is the electron coordinate, and U _{ Λ,Q }are related to the Fourier coefficients of the electronion potential [10].
For numerical implementation of the model, the above Hamiltonian needs to be represented in a suitable basis. Owing to the amorphous nature of the SiO_{ x } layers, atomistic models are of limited applicability. Furthermore, the use of an effective mass theory simplifies the electronic model considerably. For a quasionedimensional multilayer system, where quantization appears only in the vertical (growth) direction, the corresponding basis functions have the form:
where is the envelope basis function for discrete spatial (layer) index i (longitudinal) and transverse momentum k _{∥} = (k _{ x }, k _{ y }), and is the Bloch function of bulk band n, centered on k _{0}. In the case of a system with large transverse extension, the envelope basis function can be written as
where r _{∥} = (x, y), is the crosssectional area, and χ _{ i }is the localized longitudinal envelope function basis element. For the latter, finite element shape functions are a popular choice [8, 11]. Here, we will use a simple finite difference basis equivalent to a separate single band tightbinding approach for each band [12–14]. In the above basis, the fermion field operators for the charge carriers are represented via
where ĉ ^{†}, and ĉ are single fermion creation and annihilation operators.
The representation of the model system Hamiltonian in the above basis is now obtained in standard second quantization. For the isolated electronic system, we find
with the matrix elements
where , α = x, y, z are the effective mass components of band n. For the stepfunction shape element of the finite difference approximation, the above expressions acquire the form:
where
and Δ is the grid size, which is kept constant for equivalence to the single band nearestneighbor tightbinding formulation, where the above Hamiltonian is written as
defining the interlayer or hopping elements t, and the intralayer or onsite elements D. In the same way, the representation of the electronphoton Hamiltonian (6) in the realspace effective mass basis (13) is obtained:
where the matrix element for interband transitions (n ≠ m) is obtained from a k · ptype approximation [8]:
with the Bloch function momentum matrix element
where Ω denotes the unitcell volume, and
In the finite difference representation, this last factor becomes
and the final representation of the electronphoton interaction Hamiltonian takes the form:
The effectivemass Hamiltonian for electronphonon interaction is obtained from (12) in analogy to the electronphoton interaction:
with
The explicit form of the interaction term still depends via U _{ Λ,Q }on the specific phonon modes considered and will be detailed in the section on the model implementation.
Green's functions, self energies, and quantum kinetic equations
Within the nonequilibrium Green's function theory of quantum optics and transport in excited semiconductor nanostructures, physical quantities are expressed in terms of quantum statistical ensemble averages of single particle operators for the interacting quasiparticles introduced above, namely, the fermion field operator for the charge carriers, the quantized photon field vector potential Â for the photons, and the ionic displacement field for the phonons. The corresponding Green's functions are
where 〈...〉_{ C } denotes the contourordered operator average peculiar to nonequilibrium quantum statistical mechanics [15, 16] for arguments 1 = (r _{1}, t _{1}) with temporal components on the Keldysh contour [16].
The Green's functions follow as the solutions to corresponding Dyson's equations [9, 17–19],
Where , and are the propagators for noninteracting electrons, photons, and phonons, respectively, and ↔ denotes transverse and boldface tensorial quantities. The electronic selfenergy Σ encodes the renormalization of the charge carrier Green's functions because of the interactions with photons and phonons, i.e., generation, recombination, and relaxation processes. Charge injection and absorption at contacts is considered via an additional boundary selfenergy term reflecting the openness of the system. The photon and phonon selfenergy tensors, and Π ^{p}, describe the renormalization of the optical and vibrational modes, leading to phenomena such as photon recycling or the phonon bottleneck responsible for hot carrier effects. The selfenergies can be derived either via perturbative methods using a diagrammatic approach or a Wick factorization or using variational derivatives. Again, for numerical evaluation, quantum kinetic equations and selfenergies need to be represented in a suitable basis. For this purpose, the above Green's functions are replaced by the expressions in terms of the corresponding basis operators:
where for the bosonic degrees of freedom, the present form is suitable for the description of bulk propagators. Henceforth, any renormalizing effect of the electronic system on the photons and phonons is neglected, i.e., the coupling to the bosons corresponds to the connection to corresponding equilibrium reservoirs. While this treatment is generally a good approximation in the case of phonons, it is valid for the coupling to the photonic systems only in the case of low absorption, i.e., weak coupling or very short absorber length. The equilibrium propagators for noninteracting photons and phonons in isotropic media have the common form (α = γ, p):
In the above expressions, denotes the occupation of the respective equilibrium boson modes, with the phonon occupation given by the BoseEinstein distribution at lattice temperature T:
and the photon occupation related to the modal photon flux via
where is the speed of the light in the active medium. The modal photon flux, in turn, is given by the modal intensity of the EM field as .
The use of the equilibrium boson propagators implies that only the electronic Dyson equations are solved. In the chosen discrete realspace basis, the components of the steadystate Dyson and Keldysh equations for electronic Greens functions are turned into a linear system[20] (v = k _{∥}; E)
for each total energy, E, and transverse momentum, k _{∥}. There are two types of selfenergies in the above equations. The terms Σ ^{·B}denote the contact selfenergy, which, in this case, is obtained by electronic modematching to the bulk Bloch states of the flatband contact region[21]. The components Σ ^{·I}are due to the interactions of electrons with photons and phonons. The expressions for these interaction selfenergies are determined as the Fock term within manybody perturbation theory on the level of a selfconsistent Born approximation, and using the equilibrium boson propagators are obtained in the following form (α = γ, p)
and
where
Since the principal value integral in the expression for the retarded selfenergy corresponds to the real part of the latter and thus to the renormalization of the electronic structure, which is both small and irrelevant for the photovoltaic performance, it is neglected in the numerical implementation. A further approximation is made by neglecting the offdiagonal terms in the band index, which means that only incoherent interband and subband polarization is considered [18].
Once the Green's functions and selfenergies have been determined via selfconsistent solution of Equations 4548 and 49, 50, they can be directly used for expressing the physical quantities that characterize the system, such as charge carrier and current densities as well as the rates for the different scattering processes.
Microscopic optoelectronic conservation laws and scattering rates
The macroscopic balance equation for a photovoltaic system is the steadystate continuity equation for the charge carrier density:
where j _{c} is the particle current density, is the generation rate, and is the recombination rate of carrier species c[22]. In the microscopic theory, the divergence of the electron (particle) current is given by [15, 16]:
If the integration is restricted to either conduction or valence bands, then the above equation corresponds to the microscopic version of (52) and provides on the RHS the total local interband scattering rate. The total interband current is obtained by integrating the divergence over the active volume, and is equivalent to the total global transition rate and, via the Gauss theorem, to the difference of the interband currents at the boundaries of the interacting region. Making use of the cyclic property of the trace, it can be expressed in the form:
with units [R] = s ^{1}. If we are interested in the interband scattering rate, then we can neglect in Equation 54 the contributions to the selfenergy from intraband scattering, e.g., via interaction with phonons, lowenergy photons (free carrier absorption), or ionized impurities, since they cancel upon energy integration over the band. Since inequivalent conduction band valleys may be described by different bands, the corresponding intervalley scattering process has also an interband character with a non vanishing rate, as long as only one of the valleys is considered in the rate evaluation. Furthermore, if selfenergies and Green's functions are determined selfconsistently as they must be done to guarantee current conservation, the Green's functions are related to the scattering selfenergies via the Dyson equation for the propagator and the Keldysh equation for the correlation functions as given in Equations 4548, and will thus be modified because of the intraband scattering. In the present case of indirect optical transitions, the Greens functions entering the rate for electronphoton scattering between the Γ bands are the solutions of Dyson equations with an intervalley phononscattering selfenergy and may thus contain contributions from the Xvalleys. In the same way, the Γ _{ c }Greens functions entering the electronphonon Γ _{ c } X scattering rate contain a photogenerated contribution. By this way, indirect, phononassisted optical transitions are enabled.
Implementation for SiSiO_{ x }superlattice absorbers
Electronic structure model
Within the effective mass approximation (EMA) for silicon chosen in this study, the electrons are described by a multivalley picture with different values for transverse and longitudinal effective masses, similar to [23]. However, for simplicity, in the case of transverse X valleys (X _{∥}), the anisotropy in the transverse mass is neglected, and an average value is used. The virtual Γ states used in the indirect transitions are described by an additional mass. The holes are modeled by two decoupled single bands with different effective masses corresponding to heavy and light holes. Thus, in total, five bands are used for describing the electronic structure, three for the electrons (X _{∥}, X _{⊥}, Γ _{ c }), and two for the holes (Γ _{ vl }, Γ _{ vh }). The band parameters used in the simulations are listed in Table 1. The approximate value for the oxide effective mass is adopted from [3, 24]. For each band, a set of Green's functions are computed from the corresponding decoupled Dyson and Keldysh equations. In the computation of physical quantities such as electron and hole densities as well as the corresponding current densities, the summation over all conduction or valence bands needs to be performed, e.g., for the electron density:
where f _{ b } denotes the degeneracy of the conduction bands, which is , and . Similarly, the electron current in terms of the Green's functions reads
For the chosen model of the bulk band structure, the total radiative rate is
and the intervalley phonon scattering rate reads
Interactions
Optical transitions are assumed to take place only at the center of the Brillouin zone, i.e., between Γ _{ v } and virtual Γ _{ c } states, the latter being (de)populated via phonon scattering from (to) the X valleys, which carry the photocurrent. All other transition channels, e.g. electronphonon scattering in the valence band before photon absorption, are neglected at this stage. The momentum matrix element in the electronphoton coupling is thus to be taken between the Γ _{ v } and Γ _{ c } bands at k _{0} = 0. The interaction matrix elements in (27) are evaluated using an average effective coupling for both light and heavy holes:
with the Kane energy E _{P} ≈ 10 eV [25].
Four different types of phonons are used in this study to describe both carrier relaxation as well as phononassisted optical transitions. For the relaxation process, X  X intervalley scattering mediated by different optical and acoustic modes is used for the electrons, and scattering with nonpolar optical phonon for the holes. Further broadening is added for both carrier species through acoustic phonon intravalley scattering. Finally, the momentum transfer for the indirect optical transitions is mediated via Γ _{ c }  X intervalley scattering. For all processes, the electronphonon interaction is described by the deformation potential picture, where the coupling elements in (33) have the general form [25]:
where D is the deformation potential, and ρ is the density of the semiconductor material. For intravalley scattering of electrons by longitudinal acoustic phonons, the coupling is given by [12]:
where c _{ s } is the speed of sound in the semiconductor, and the interaction is treated as being elastic, i.e., no energy is transferred. In this case, the phonon occupation can be approximated as
which leads to a product of coupling and occupation that does not depend on momentum. As a consequence, the sum over q _{ z } of the exponential in (33) yields a delta function in space:
where L = N _{ z } Δ is the thickness of the device with N _{ z } model layers, resulting in the local selfenergy (b = Γ _{ c }, X):
The parameters for intravalley scattering used in the numerical simulation are ρ = 2329 g/cm^{3}, c _{ s } = 9.04 × 10^{5} cm/s, and D _{ ac } = 8.9322 eV [14].
For X  X and Γ  X intervalley scattering, the coupling reads
where σ labels the phonon mode, and K denotes the momentum transfer required for the scattering between two valleys. Using a constant, modespecific coupling strength, the selfenergy acquires the diagonal form:
In the above expression, b = b' for gtype X  X intervalley scattering and b = b' for ftype X  X scattering as well as for Γ  X scattering. The deformation potentials and phonon energies for the different optical and acoustic modes participating in the intervalley scattering process are given in Table 2.
Finally, intravalley scattering of holes via interaction with nonpolar optical phonons is described by the coupling term [25]:
providing the selfenergy (b = Γ _{ v,lh/hh })
For the numerical simulation, an optical deformation potential of D _{ op } = 10^{9} eV/cm and a constant phonon energy ħΩ _{op} = 60 meV are used.
Numerical results and discussion
Model system
The model system under investigation is shown schematically in Figure 1. It consists of a set of four coupled quantum wells of six monolayer (ML) width with layers separated by oxide barriers of 3ML thickness, embedded in the intrinsic region of a Si pin diode. The thickness of the doped layers is 50 ML, while the total length of the iregion amounts to 154 ML. The monolayer thickness is half the Si lattice constant, i.e., Δ = 2.716 Å. The doping density is N _{d} = 10^{18} cm^{3} for both electrons and holes. This composition and doping leads to the band diagram shown in Figure 2.
Density of states
Insertion of the oxide barriers leads to an increase of the effective band gap in the central region of the diode from 1.1 to ~ 1.3 eV, as seen in Figure 3, which shows the transverse momentumintegrated local density of states. In the actual situation of strong band bending, quantization also occurs in the form of notch states in front of the barriers. The density of states at minority carrier contacts is additionally depleted because of the imposition of closedsystem boundary conditions that prevent the formation of a dark leakage current under bias.
The density of states component at zero transverse momentum displayed in Figure 4 allows the identification of the confined states in the different quantum wells, which are considerably localized because of the large internal field, however, with finite overlap between neighboring wells in the case of the higher states. The ground state is split because of the different effective masses of the charge carriers, the effect being more pronounced for the electrons.
Generation and photocurrent spectrum
The spectral rate of carrier generation in the confined states under illumination with monochromatic light at photon energy E _{ γ } = 1.65 eV and intensity I _{ γ } = 10 kW/m^{2}, is shown in Figure 5. At this photon energy, both the lowest and the second minibands are populated. The photocurrent originating in this excitation is shown in Figure 6. Current flows also in both first and second minibands, i.e., over the whole spectral range of generation, which means that relaxation due to scattering is not fast enough to confine transport to the band edge. However, transport of photocarriers is strongly affected by the inelastic interactions, and is the closest to the sequential tunneling regime.
Conclusions
In this article, an adequate theoretical description of photogeneration and transport in SiSiO_{ x } superlattice absorbers was presented. Based on quantum kinetic theory, the formalism allows a unified approach to both quantum optics and inelastic quantum transport and is thus able to capture pivotal features of photogeneration and photocarrier extraction in Sibased coupled quantum well structures, such as phononassisted optical transitions and fielddependent transport in superlattice states. Owing to the microscopic nature of the theory, energyresolved information can be obtained, such as the spectra for photogeneration rate and photocurrent density, which shows that in the case of high internal fields, excess charge is transported via sequential tunneling in the miniband where it is generated.
Abbreviations
 EMA:

effective mass approximation
 NEGF:

nonequilibrium Green's function.
References
Green MA: Potential for low dimensional structures in photovoltaics. J Mater Sci Eng 2000, 74(1–3):118–124. 10.1016/S09215107(99)005462
Green MA: Third generation photovoltaics: Ultrahigh conversion efficiency at low cost. Prog Photovolt: Res Appl 2001, 9: 123. 10.1002/pip.360
Jiang CW, Green MA: Silicon quantum dot superlattices: Modeling of energy bands, densities of states, and mobilities for silicon tandem solar cell applications. J Appl Phys 2006, 99(11):114902. 10.1063/1.2203394
Wacker A: Semiconductor superlattices: a model system for nonlinear transport. Phys Rep 2002, 357: 1. 10.1016/S03701573(01)000291
Aeberhard U, Morf R: Microscopic nonequilibrium theory of quantum well solar cells. Phys Rev B 2008, 77: 125. 343 343 10.1103/PhysRevB.77.125343
Aeberhard U: A Microscopic Theory of Quantum Well Photovoltaics. In Ph.D. thesis. ETH Zurich; 2008.
Steiger S, Veprek RG, Witzigmann B: Electroluminescence from a quantumwell LED using NEGF. Proceedings  2009 13th International Workshop on Computational Electronics, IWCE 2009 2009.
Steiger S: Modeling NanoLED. In Ph.D. thesis. ETH Zurich; 2009.
Schäfer W, Wegener M: Semiconductor Optics and Transport Phenomena. Springer, Berlin; 2002.
Mahan GD: ManyParticle Physics. 2nd edition. Plenum, New York; 1990.
Kubis T, Yeh C, Vogl P, Benz A, Fasching G, Deutsch C: Theory of nonequilibrium quantum transport and energy dissipation in terahertz quantum cascade lasers. Phys Rev B 2009, 79: 195323. 10.1103/PhysRevB.79.195323
Lake R, Klimeck G, Bowen R, Jovanovic D: Single and multiband modelling of quantum electron transport through layered semiconductor devices. J Appl Phys 1997, 81: 7845. 10.1063/1.365394
Henrickson LE: Nonequilibrium photocurrent modeling in resonant tunneling photodetectors. J Appl Phys 2002, 91: 6273. 10.1063/1.1473677
Jin S: Modeling of Quantum Transport in NanoScale MOSFET Devices. In Ph.D. thesis. School of Electrical Engineering and Computer Science College of Engineering, Seoul National University; 2006.
Kadanoff LP, Baym G: Quantum Statistical Mechanics. Benjamin, Reading, Mass; 1962.
Keldysh L: Diagram technique for nonequilibrium processes. Sov PhysJETP 1965, 20: 1018.
Henneberger K, Haug H: Nonlinear optics and transport in laserexcited semiconductors. Phys Rev B 1988, 38: 9759–9770. 10.1103/PhysRevB.38.9759
Pereira M, Henneberger K: Green's function theory for semiconductorquantumwell laser spectra. Phys Rev B 1996, 53: 16. 485 485 10.1103/PhysRevB.53.16485
Pereira M, Henneberger K: Microscopic theory for the influence of coulomb correlations in the lightemission properties of semiconductor quantum wells. Phys Rev B 1998, 58: 2064. 10.1103/PhysRevB.58.2064
In steady state, the Green's functions depend only on the difference τ = t  t' of the realtime variables, which is Fouriertransformed to energy
For an explicit derivation of the contact selfenergy in the effectivemass tightbinding model, see, e.g., [12]
The dimensions are those of a volume rate, = m ^{3} s ^{1}
Jin S, Park YJ, Min HS: A threedimensional simulation of quantum transport in silicon nanowire transistor in the presence of electronphonon interactions. J Appl Phys 2006, 99: 123719. 10.1063/1.2206885
While the validity of the EMA for the oxide is debatable, moderate variations of the parameter should not have a strong impact on the results, since the dominant dependence is on the barrier energy
Ridley BK: Quantum Processes in Semiconductors. Oxford Science Publications; 1993.
Hamaguchi C: Basic Semiconductor Physics. Springer, Berlin; 2001.
Acknowledgements
The financial support for this study was provided by the German Federal Ministry of Education and Research (BMBF) under Grant No. 03SF0352E.
Author information
Authors and Affiliations
Corresponding author
Additional information
Competing interests
The author declares that he has no competing interests.
Authors' contributions
UA carried out all of the work related to this manuscript.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 2.0 International License (https://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
About this article
Cite this article
Aeberhard, U. Theory and simulation of photogeneration and transport in SiSiO_{ x } superlattice absorbers. Nanoscale Res Lett 6, 242 (2011). https://doi.org/10.1186/1556276X6242
Received:
Accepted:
Published:
DOI: https://doi.org/10.1186/1556276X6242
Keywords
 Solar Cell Device
 Quantum Kinetic Equation
 Intervalley Scattering
 Momentum Matrix Element
 Indirect Optical Transition